Download presentation

Presentation is loading. Please wait.

Published byJosue Boykin Modified about 1 year ago

1
1T. Kim Parnell; May 3, 1999 Fracture Mechanics Overview & Basics T. Kim Parnell, Ph.D., P.E. May 3, 1999

2
2T. Kim Parnell; May 3, 1999 Motivation Brittle failure at low stress in low- strength steels –WWII era Liberty Ships Welded structures Ductile/Brittle transition temperature too high The occurrence of failure at low stress in high-strength materials spurred Fracture Mechanics further NBS economic study in 1978 estimated the cost of fracture at $119 Billion in the U.S. (about 4% of the GNP) Brittle failure at low stress in low- strength steels –WWII era Liberty Ships Welded structures Ductile/Brittle transition temperature too high The occurrence of failure at low stress in high-strength materials spurred Fracture Mechanics further NBS economic study in 1978 estimated the cost of fracture at $119 Billion in the U.S. (about 4% of the GNP) T.L.Anderson, “Fracture Mechanics” p. 3

3
3T. Kim Parnell; May 3, 1999 Fracture v Strength Criteria

4
4T. Kim Parnell; May 3, 1999 Historical Development A.A. Griffith work on brittle fracture G.R. Irwin extended Griffith’s work to ductile materials A.A. Griffith work on brittle fracture G.R. Irwin extended Griffith’s work to ductile materials

5
5T. Kim Parnell; May 3, 1999 Work of Griffith A. A. Griffith started his work in around the 1920s. At this time, it was accepted that the theoretical strength of a material was taken to be E/10, where E is Young's Modulus for the particular material. He was only considering elastic, brittle materials, in which no plastic deformation took place. However, it was observed that the true values of critical strength was as much as 1000 times less than this predicted value, and Griffith wished to investigate this discrepancy. He discovered that there were many microscopic cracks in every material which were present at all times. He hypothesized that these small cracks actually lowered the overall strength of the material because as a load is applied to these cracks, stress concentration is experienced. A. A. Griffith started his work in around the 1920s. At this time, it was accepted that the theoretical strength of a material was taken to be E/10, where E is Young's Modulus for the particular material. He was only considering elastic, brittle materials, in which no plastic deformation took place. However, it was observed that the true values of critical strength was as much as 1000 times less than this predicted value, and Griffith wished to investigate this discrepancy. He discovered that there were many microscopic cracks in every material which were present at all times. He hypothesized that these small cracks actually lowered the overall strength of the material because as a load is applied to these cracks, stress concentration is experienced.

6
6T. Kim Parnell; May 3, 1999 Work of Irwin G. R. Irwin, in the 1950s, began to see how the theory outlined by Griffith would apply to ductile materials. He determined that there was also a certain energy from plastic deformation that had to be added to the strain energy originally considered by Griffith in order for the theory to work for ductile materials. Irwin developed the concept of the strain energy release rate. G. R. Irwin, in the 1950s, began to see how the theory outlined by Griffith would apply to ductile materials. He determined that there was also a certain energy from plastic deformation that had to be added to the strain energy originally considered by Griffith in order for the theory to work for ductile materials. Irwin developed the concept of the strain energy release rate.

7
7T. Kim Parnell; May 3, 1999 Concepts & Principles Crack tip stress distribution –1/ r singularity at the crack tip (LEFM) Energy Release Rate is related to the Stress Intensity Factor Condition at the crack tip is characterized by the Stress Intensity Factor, K I Fracture toughness is a material property, K Ic. Crack tip stress distribution –1/ r singularity at the crack tip (LEFM) Energy Release Rate is related to the Stress Intensity Factor Condition at the crack tip is characterized by the Stress Intensity Factor, K I Fracture toughness is a material property, K Ic.

8
8T. Kim Parnell; May 3, 1999 Three Modes of Cracking –Mode I - opening mode –Mode II - in-plane shearing/sliding mode –Mode III - out-of-plane shearing/tearing mode –Mode I - opening mode –Mode II - in-plane shearing/sliding mode –Mode III - out-of-plane shearing/tearing mode Deal with Mode I most frequently Kim Parnell: Sketch from p.8 Kim Parnell: Sketch from p.8

9
9T. Kim Parnell; May 3, 1999 Stress Concentration K -> 3 for circular hole in infinite plate with tension Stress Concentration Factor Maximum Stress

10
10T. Kim Parnell; May 3, 1999 Crack Tip Stresses Ex: (ksi- in, MPa- m)

11
11T. Kim Parnell; May 3, 1999 Some Applications of Fracture Mechanics Remaining life as a function of crack size Crack size that can be tolerated (critical crack size) Time for a crack to grow from an initial size to the critical size (inspection interval) Remaining life as a function of crack size Crack size that can be tolerated (critical crack size) Time for a crack to grow from an initial size to the critical size (inspection interval)

12
12T. Kim Parnell; May 3, 1999 Test Techniques for Fracture Properties Compact Tension (CT) specimen Charpy impact specimen Compact Tension (CT) specimen Charpy impact specimen

13
13T. Kim Parnell; May 3, 1999 Stress Intensity Factors for CT

14
14T. Kim Parnell; May 3, 1999 Miniature Specimens Trend: Development of techniques using miniature specimens Example: Small Punch procedure for generating constitutive properties & fracture toughness Trend: Development of techniques using miniature specimens Example: Small Punch procedure for generating constitutive properties & fracture toughness

15
15T. Kim Parnell; May 3, 1999 Piping Design: Leak Before Break Criteria Desirable for pipe to be able to grow a crack through-wall (leak) without unstable crack growth (break). Leak provides an opportunity to detect the crack before it becomes long enough to be critical. Desirable for pipe to be able to grow a crack through-wall (leak) without unstable crack growth (break). Leak provides an opportunity to detect the crack before it becomes long enough to be critical.

16
16T. Kim Parnell; May 3, 1999 Pipeline-Unstable Crack Growth 16-inch underground natural gas line 300 psi internal pressure Poor quality welds (ERW pipe) Fast fracture of a 40-ft. section after initial weld defects grew through fatigue to critical size Resulting fire & explosions demolished the plant 16-inch underground natural gas line 300 psi internal pressure Poor quality welds (ERW pipe) Fast fracture of a 40-ft. section after initial weld defects grew through fatigue to critical size Resulting fire & explosions demolished the plant

17
17T. Kim Parnell; May 3, 1999 Fatigue Growth Cyclic stress intensity factor Paris law Integrate to get Cycles to failure Cyclic stress intensity factor Paris law Integrate to get Cycles to failure

18
18T. Kim Parnell; May 3, 1999 Fatigue Fracture Surface

19
19T. Kim Parnell; May 3, 1999 Conclusions Cracks are everywhere, it is just a matter of how large! Fracture design criteria are required more often in modern design More efficient designs with lower factors of safety drive this trend Cracks are everywhere, it is just a matter of how large! Fracture design criteria are required more often in modern design More efficient designs with lower factors of safety drive this trend

20
20T. Kim Parnell; May 3, 1999 Selected References: Fracture Mechanics Broek, David (1982). Elementary Engineering Fracture Mechanics, 3rd Ed., Martinus Nijhoff Publishers. Anderson, T.L. (1991). Fracture Mechanics: Fundamentals and Applications, CRC Press. Dieter, George, E. (1976). Mechanical Metallurgy, 2nd Ed., McGraw-Hill. ASTM E399-83, (1983). “Standard Test Method for Plane-Strain Fracture Toughness of Metallic Materials.”, Philadelphia. ASTM E813-87, (1987). “Standard Test Method for J IC, a Measure of Fracture Toughness”, Philadelphia. ASTM E , (1987). “Standard Test Method for Determining J-R Curves”, Philadelphia. Broek, David (1982). Elementary Engineering Fracture Mechanics, 3rd Ed., Martinus Nijhoff Publishers. Anderson, T.L. (1991). Fracture Mechanics: Fundamentals and Applications, CRC Press. Dieter, George, E. (1976). Mechanical Metallurgy, 2nd Ed., McGraw-Hill. ASTM E399-83, (1983). “Standard Test Method for Plane-Strain Fracture Toughness of Metallic Materials.”, Philadelphia. ASTM E813-87, (1987). “Standard Test Method for J IC, a Measure of Fracture Toughness”, Philadelphia. ASTM E , (1987). “Standard Test Method for Determining J-R Curves”, Philadelphia.

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google